All rights reserved. This book or any part thereof may not be reproduced, stored in aretrieval system, or transmitted in any form or by any means, electronic, mechanical,photocopying, recording, or otherwise, without prior written permission of the publisher.Editor: Arinne DicksonProduction: Eric PrzybylskiPrinted in CanadaTable of Contents Contributors vii Acknowledgments ix Introduction x1 A Comparison of Metals, Ceramics, and Polymers 12 Physical Properties and Biocompatibility 123 Color and Appearance 244 Gypsum Products 375 Surface Phenomena and Adhesion to Tooth Structure 626 Polymers and Polymerization 747 Impression Materials 908 Polymeric Restorative Materials 1139 Dental Cements 13210 Abrasion, Polishing, and Bleaching 15611 Structure and Properties of Metals and Alloys 16512 Dental Amalgams 17513 Precious Metal Casting Alloys 19214 Alloys for Porcelain-Fused-to-Metal Restorations 20015 Dental Porcelain 21016 Base Metal Casting Alloys 22517 Casting 23918 Soldering, Welding, and Electroplating 249
19 High-Temperature Investments 25820 Waxes 26721 Orthodontic Wires 27122 Endodontic Materials 28723 Implant and Bone Augmentation Materials 294 Appendix A Tabulated Values of Physical and Mechanical Properties 309 Appendix B Biocompatibility Tests 391 Appendix C Periodic Chart of the Elements 393 Appendix D Units and Conversion Factors 394 Appendix E Answers to Study Questions 395ContributorsKenzo Asaoka, PhDProfessor and ChairDepartment of Dental EngineeringSchool of DentistryUniversity of TokushimaTokushima, JapanCh 19 • High-Temperature InvestmentsRaymond L. Bertolotti, DDS, PhDClinical Professor of Restorative DentistrySchool of DentistryUniversity of CaliforniaSan Francisco, CaliforniaCh 14 • Alloys for Porcelain-Fused-to-Metal RestorationsWilliam A. Brantley, PhDProfessorSection of Restorative Dentistry, Prosthodontics, and EndodonticsCollege of DentistryOhio State UniversityColumbus, OhioCh 21 • Orthodontic WiresGordon Christensen, DDS, MSD, PhDSenior ConsultantClinical Research AssociatesProvo, UtahLongevity of Restorations
Richard G. Earnshaw, PhD, MDScHonorary AssociateFaculty of DentistryUniversity of SydneySydney, AustraliaCh 4 • Gypsum ProductsGerald N. Glickman, DDS, MS, MBAProfessor and ChairmanDepartment of EndodonticsDirector, Graduate Program in EndodonticsSchool of DentistryUniversity of WashingtonSeattle, WashingtonCh 22 • Endodontic MaterialsEugene F. Huget, BS, DDS, MSProfessorDepartment of Restorative DentistryCollege of DentistryUniversity of TennesseeMemphis, TennesseeCh 16 • Base Metal Casting AlloysAbraham Jarjoura, DDSDepartment of Biologic and Materials SciencesSchool of DentistryUniversity of MichiganAnn Arbor, MichiganCh 22 • Endodontic MaterialsDavid H. Kohn, PhDAssociate ProfessorDepartment of Biologic and Materials SciencesSchool of DentistryDepartment of Biomedical EngineeringSchool of EngineeringUniversity of MichiganAnn Arbor, MichiganCh 23 • Implant and Bone Augmentation MaterialsJ. Rodway Mackert, Jr, DMD, PhDProfessor of Dental MaterialsDepartment of Oral RehabilitationSchool of DentistryMedical College of GeorgiaAugusta, GeorgiaCh 1 • A Comparison of Metals, Ceramics, and PolymersCh 2 • Physical Properties and Biocompatibility
Peter C. Moon, MS, PhDProfessor of Restorative DentistrySchool of DentistryMedical College of VirginiaVirginia Commonwealth UniversityRichmond, VirginiaCh 11 • Structure and Properties of Metals and AlloysAnn-Marie L. Neme, DDS, MSAssociate ProfessorDepartment of Restorative DentistrySchool of DentistryUniversity of Detroit MercyDetroit, MichiganCh 8 • Polymeric Restorative MaterialsOsamu Okuno, PhDProfessor and ChairDivision of Biomaterials ScienceGraduate School of DentistryTohoko UniversitySendai, JapanCh 19 • High-Temperature InvestmentsStephen T. Rasmussen, PhDResearch AssociateDepartment of Biologic and Materials SciencesSchool of DentistryUniversity of MichiganAnn Arbor, MichiganCh 18 • Soldering, Welding, and ElectroplatingDennis C. Smith, MSc, PhD, FRISProfessor EmeritusFaculty of DentistryUniversity of TorontoToronto, Ontario, CanadaCh 9 • Dental CementsKenneth W. Stoffers, DMD, MSClinical Associate ProfessorDepartment of Cariology, Restorative Sciences, and EndodonticsSchool of DentistryUniversity of MichiganAnn Arbor, MichiganClinical Decision-Making ScenariosJohn A. Tesk, BS, MS, PhDCoordinatorBiomaterials Program Polymers DivisionNational Institute of Standards and TechnologyGaithersburg, Maryland
AcknowledgmentsI would like to thank the many contributors to the third edition who took the time andused their expertise to keep this book current in a field that has seen many changes inrecent years. Several contributors to the second edition are also recognized for theirvaluable contributions: Dr Pui L. Fan, Dr Evan H. Greener, Carole L. Groh, Dr Valerie A.Lee, and Dr Mathijs M. A. Vrijhoef.I appreciate the many people who contributed data to the biomaterials properties tables,especially Drs Hal OKray and Abe Jarjoura, who provided major additions to the data onrestorative and impression materials, respectively. Chris Jung contributed many excellentillustrations, and Elizabeth Rodriguiz was invaluable in preparing the manuscript. Finally,I want to acknowledge the staff at Quintessence for their expert assistance in helping meprepare the book for publication.IntroductionIn revising this book for a third edition, the current situation confronting academic dentalmaterials was considered. On one hand, dental materials is one of the most popularsubjects among those who pursue continuing education seminars and read the dentalliterature. On the other hand, most dental students think of dental materials as a basicscience course, filled with facts and concepts that have little application to clinicaldentistry. A perusal of current dental textbooks on restorative dentistry andprosthodontics reveals that such texts cover much of the subject matter formerly taughtonly in dental materials courses. This sign of our success in integrating dental materialsinto dental education and research is also a sign that the dental materials curriculum mustcontinue to evolve to maintain its vital position as an intellectual leader in dentaleducation. More and more of the traditional approach simply will not do for this thirdedition. Instead, we must seize the opportunity to move the field of dental materialseducation forward to tackle two major challenges in dentistry: the proliferation ofproducts and techniques and the information explosion in science and technology. Therecent proliferation of dental products may lead to improved patient care, but keeping upwith the new technology is a challenge to dental materials specialists and educators.Dental materials textbooks have evolved significantly over the past century. An earlytextbook on dental materials provided recipes for a handful of materials (three cements,amalgam alloys, gold foil, vulcanized rubber, and gold casting materials) and emphasizedformulation, techniques, and crude testing. Then came the research and developmentperiod, when dental materials properties were optimized by the dentist according to theresults of laboratory testing and ADA standards were developed. Dental materials havebeen further refined to offer simpler techniques for clinicians and to meet the increasingesthetic demands of middle-class patients in developed countries.Another dimension to proliferation is the large number of products and techniquesavailable for each type of material, which only intensifies the need for dentists to staycurrent with the literature. To ease this burden, publications such as Clinical ResearchAssociates Newsletter, Dental Advisor, and Reality compile new information and providemonthly updates for dental practitioners. Perhaps the greatest drawback of proliferation isthat many new materials are not sufficiently tested prior to full-scale marketing, therebyincreasing the risk of clinical failures.As a result of this product explosion, dental materials education has an opportunity to
become a more integral part of the overall curriculum, but to do so it must revise itsapproach to teaching. A long-standing problem is that dental materials courses aregrouped with basic sciences, which tends to encourage memorization of facts rather thanunderstanding of clinical application. A new approach (Fig 1)would be more pragmatic, integrating problem-based learning and evidence-baseddentistry with the traditional overview of clinical materials and materials scienceconcepts, which is still important. Table 1 Table 1 Longevity of Restorations Commonly Used in Dentistry Gordon J. Christensen, DDS, MSD, PhDMaterial /Estimated Indications Contraindications Strengths WeaknesseslongevityAmalgam, Incipient, Large intracoronal Good marginal Objectionablesilver /14 y moderate- restorations (cusp seal; strength; color; stains tooth; sized, and replacement); longevity; marginal some large endodontically manipulability; breakdown; lesions in treated teeth cariostatic activity alleged health adolescents and challenges adultsCast gold Large lesions; Adolescents; high Reproduces Time required for(inlays, teeth requiring caries activity; anatomy well; placement; highonlays, and additional persons who object to onlays and fee; poorcrowns) / 20 strength; teeth gold display crowns may esthetics; thermaly used in increase strength sensitivity rebuilding or of tooth; changing longevity; wears occlusion occlusally similar
to enamelCeramic Restoration of Heavy occlusal Esthetics; no Have onlycrowns /15 y teeth requiring stress; bruxism; fixed metal content moderate strength; good prosthesis longer than require resin appearance and three teeth bonding for moderate strength strengthCeramic Class 2 and 5 Teeth that are grossly Esthetic potential May create toothinlays and locations where broken down and extremely high; sensitivity ifonlays (fired high esthetics require crowns properly etched bonding agentsor pressed) / is desired tooth and are not used10 y restoration may properly; may increase strength fracture during of tooth; onlays service stronger than inlaysCompacted Initial Class 3 Periodontally Marginal Time-consuming;golds (gold and 5lesions unstable teeth; high integrity; poor estheticsfoil, for patients of caries activity; longevitypowdered all ages persons who object togold, mat gold displaygold) / 24 yCompomer / Moderate to Occlusal stress; Moderate fluoride Color degrades10 y high caries locations where color release; easy to activity; repair stability is necessary use of crowns; pediatricGlass Class 1 and 2 Areas of high esthetic High fluoride Only fairionomer / 8 y High caries need; areas of release esthetics; difficult activity; crown difficult moisture and time- repairs control consuming to placeHybrid High caries Occlusal stress; High fluoride Somewhationomer / 10 activity; repair locations where color release; tri-cured; difficult to use;y of crowns; stability is necessary sets in dark color degrades pediatric Class 1 and 2Porcelain- Teeth that Heavy occlusal Strength; good Appearance not asfused-to- require full stress; bruxism marginal fit; good as somemetal crowns coverage and acceptable to others; possible/ 20 y are subject to excellent esthetic wear of opposing heavy occlusal result teeth forces; fixed prosthesisResin Class 1 and 2 Bruxers and Esthetics; may Wear ofcomposite areas of high clenchers strengthen tooth restoration during(Class 1, 2) / esthetic need; with acid-etch service; no10 y patients concept cariostatic sensitive to activity; may metal cause tooth sensitivity if
innovation and risk. For example, dentin etching for the purpose of bonding compositematerials to dentin was highly innovative and had many risks when it was firstintroduced. The next, lower level of innovation includes major product changes in aconventional material, such as with high-copper amalgam alloys in the 1970s or hybridionomer cements in the 1990s. Decreasing levels of innovation and risk include minorproduct improvements (eg, more shades for a resin restorative material). The majority of"new products" fall into this category.Each category in the hierarchy of evidence is described below.Large-scale, long-term clinical trialsA well-designed clinical trial will have a clearly stated hypothesis about the clinicalperformance of a new material when compared with a control material. It will have alarge number of subjects to be sufficiently definitive. A good design will also reducesubjectivity by using methods such as calibration of observers, double-blind procedures,and randomization, and the institutional review board of the organization will protect thestudy participants. These studies are indicated for adoption of brand new innovations andmajor product changes.Other clinical studiesOther types of clinical study generally are not as decisive as full clinical trials, but theynevertheless provide valuable information. A cohort study would follow a group ofpatients who receive biomaterials, for instance, and record successes and failures relatedto their characteristics. Follow-up studies evaluate product longevity and causes of failurein patients who are treated in a clinic. A significant finding might be one in which aresearcher discovers a high failure rate of a new biomaterial as patients return forreplacement within a short period of time. Short-term clinical studies performed for newdental restorative materials by manufacturers are common and useful, but they miss long-term effects and less frequent problems that are usually only evident in larger groups ofpatients. Studies in this category are indicated for product improvements and newtechniques.Animal experimentsSeveral of the biocompatibility tests for new materials involve animal testing. Animaltests are valuable, but they are often difficult to interpret. Cytotoxicity screening testswith cell cultures will detect gross toxicity of a material, but subtle effects require expertinterpretation. Animal tests are required for new compositions or techniques withquestionable biocompatibility.Physical properties dataThe publication of physical properties data on new biomaterials is essential for predictingsuccessful performance, as compared with a standard material. However, since conditionsin the body are highly complex, data from laboratory tests cannot always be extrapolatedto clinical performance. For example, a new material may be strong when tested in thelaboratory, but it may deteriorate more rapidly in body fluids and thus may not be animprovement when compared with a standard material. It is important to evaluate allapplicable physical properties of a new material alongside its clinical trials. Physicalproperties data are usually necessary for minor improvements in materials, but they are
combines the strength and ductility of metal with the esthetics of dental porcelain. Aceramic or polymer base is used to insulate the pulp from a thermal-conductive metallicrestoration. A high thermal-expansion, low-strength, low-elastic-modulus polymer isreinforced with a low thermally expanding, high-strength, high-elastic-modulus ceramicfiller to form a dental resin composite material. An understanding of the advantages andlimitations of the various types of materials enables us to make selections based on thebest compromise of desired properties versus inherent limitations.Predicted Versus Actual StrengthsIt is possible to predict the strength of a material from the strengths of the individualbonds between the atoms in the material. The values of strength obtained by such aprediction are typically 1 million to 3 million pounds per square inch (psi), or about 7 to21 GPa. Actual strengths of most materials are ten to 100 times lower.Why do materials fail to exhibit the strengths one would expect from the bonds betweenatoms? Why do ceramics break suddenly without yielding, whereas metals often yieldand distort to 120% or more of their original length before fracturing? Why are polymersso much weaker and more flexible than metals and ceramics? Why do metals conductheat and electricity, whereas polymers and ceramics do not? As will be seen in thischapter, many of the answers to these questions can be understood by knowing only a fewthings about the structures of these materials. There is one key concept, for example, thatwill not only explain the tendency for ceramics to be brittle, but will also explain all ofthe methods used to strengthen ceramics. Similarly, one key concept will explain whypolymers expand about ten times as much as metals or ceramics when heated the sameamount, why polymers are generally weak, why they are ten times more flexible thanmetals or ceramics, and why they tend to absorb water and other fluids.CeramicsIntroductionConsider a block of material as depicted in Fig 1-2(a)
Fig 1-2 Stress raisers and the effect of their shape on stress concentration. (a) If no stressraiser is present, the stress is constant across cross section A. (b) If a rounded notch ispresent, the stress is constant over most of the cross section. (c) As the notch becomessharper, the stress concentration becomes greater. If this block is stretched by applying a force, F, the stress at any point on cross section Ais the same as the average stress, σave. For example, if the cross-sectional dimensions ofthe block are 1/2 in × 1/2 in = 1/4 in2 (1.27 cm × 1.27 cm = 1.61 cm2), and a force of3,000 lb (13 kN) is applied, the average stress along cross section A is 12,000 psi (83MPa). However, if a semicircular groove were machined across one side of the block ofmaterial, as depicted in Fig 1-2(b), the stress at each point across a plane passing throughthis groove would not be the same as the average stress. The stress would be constantover most of the cross section, but near the groove, the stress would suddenly rise andreach a maximum right at the edge of the groove. This phenomenon occurs around anyirregularity in a block of material. The groove or other irregularity is called a stressraiser. The stress around a stress raiser can be many times higher than the average stressin the body. The amount of increased stress depends on the shape of the stress raiser. Forexample, if the stress raiser in our block of material were a sharp notch rather than asemicircular groove, the stress would increase greatly at the tip of the sharp notch (Fig 1-2(c)). As the tip of the notch becomes smaller (ie, the notch becomes sharper), the stressconcentration at the tip of the notch becomes greater.The minute scratches present on the surfaces of nearly all materials behave as sharpnotches whose tips are as narrow as the spacing between atoms in the material. Thus, thestress concentration at the tips of these minute scratches causes the stress to reach the
Understanding the effect of stress concentration is the key to understanding the failure ofbrittle materials, such as ceramics, which influences their selection as dental materials anddictates the design of restorations fabricated from these materials.The tendency for ceramics to fail in a brittle manner at stresses that are far below thetheoretical strengths of these materials can be understood in light of the concept of stressconcentration at surface scratches and other defects. Most of the techniques forstrengthening ceramics can also be understood by virtue of this concept.* Actually, the exceeding of the theoretical strength of the material at the crack tip is anecessary but insufficient condition for crack propagation. The remaining conditioninvolves a balance between the surface energy required to form the two new surfaces ofthe crack, and the elastic strain energy arising from the applied stress. This is called theGriffith energy balance, discussion of which is beyond the scope of this book.Clinical applications of ceramicsCeramics are inherently brittle and must be used in such a way as to minimize the effectof this property. Ceramic restorations must not be subjected, for example, to large tensilestresses, to avoid catastrophic failure. A method for reducing the influence of thebrittleness of ceramics is to fuse them to a material of greater toughness (eg, metal), as isdone with porcelain-fused-to-metal (PFM) restorations. Ceramics also may be reinforcedwith dispersions of high-toughness materials, as is the case with the alumina (Al 2O3)-reinforced porcelain used in porcelain jacket crowns.Fig 1-4 Brittle fracture (arrows) of ceramic (dental porcelain) due to mismatch in thecoefficient of thermal expansion between porcelain and metal. (Photo courtesy of R. P.OConnor, DMD.)Figure 1-4 shows brittle fractures that occurred in the porcelain of two PFM crowns dueto the mismatch in thermal expansion between the porcelain and metal.
MetalsEffect of ductility on stress concentrationAs discussed in the previous section, stress raisers at the surface of a material can causethe stress in a localized region around the tip of the stress raiser to reach the theoreticalstrength of the material. When this happens in a brittle material, a crack propagatesthrough the material, resulting in fracture (see the footnote on page 3). In a ductilematerial, something happens before the theoretical strength of the material is reached atthe tip of the stress raiser that accounts for the tremendous difference in behaviorbetween, for example, a glass and a metal. As discussed previously, the magnitude of thestress concentration at the tip of a notch, surface scratch, or other stress raiser isdetermined by the sharpness of the stress raiser. If a sharp notch or scratch is present inthe surface of a brittle material, the stress concentration around this notch would besomething like that shown in Fig 1-5(a).Fig 1-5 Rounding or blunting of stress raisers that occurs in ductile materials. Stressconcentration is self-limiting in ductile materials because the region under greatest stress,the tip of the sharp stress raiser (a), yields to round or blunt the stress raiser and lower thestress (b).
If a stress raiser is present in a ductile metal, however, the material at the tip of the stressraiser deforms under stress so the sharp notch becomes a rounded groove, as shown in Fig1-5(b). Because the tip of the stress raiser is now rounded rather than sharp, the stressconcentration at the tip of this stress raiser is much lower. There are two important factsto recognize in this process:1. As with brittle materials, the actual strengths of ductile materials are many times lessthan those predicted from strengths of bonds between atoms.2. Unlike the behavior around the notch in a brittle material, the stress concentrationblunts the sharp tip of the stress raiser, thus lowering the stress concentration effect.Mechanism of ductile behaviorWhat, then, is responsible for the ductile behavior of a metal? Consideration of what ishappening on an atomic level provides insights into the difference between brittlematerials and ductile ones. A schematic of the arrangement of atoms in a piece of metal isshown in Fig 1-6.Fig 1-6 Tensile stress on a piece of material can be considered stress normal (n)(perpendicular) to plane A-A′, together with stress parallel (s) to plane A-A′. The stressparallel to plane A-A′ tends to cause the atoms along the plane to slide (shear) past eachother.
If this piece of metal is subjected to a tensile stress as shown, this stress can be resolvedinto two components when considered relative to the plane A-A′. One component tends tomove the rows of atoms on either side of the plane A-A′ apart from each other, and theother component tends to cause the planes to slide past one another along the plane A-A′.The component of the stress that tends to cause the planes to slide past one another is theone that causes a material to deform plastically. Scientists are able to calculate, from thebond strengths between the atoms, the stresses that would be required to make one planeof atoms slide past another plane; these stresses are 100 or more times higher than thoseactually observed. If, however, the bonds were to break one at a time and re-formimmediately with the adjacent atom, one plane could move past the other at very lowstress levels.The mechanism of this process is shown in Fig 1-7.
Fig 1-7 Figure 1-7 (a) through (f) show how the shearing stress can cause a dislocation topass through the network of atoms, breaking only one row of bonds at a time. For theatoms along plane A-A′ to slide past one another all at once would require enormousstress. The fact that metals yield to stresses much lower than expected is explained by thebreaking of only one row of bonds (perpendicular to the page) at a time. Figure 1-7 (a) through (f) show how, by breaking and re-forming bonds, an extra plane ofatoms can move along plane A-A′ until this "ripple" in the crystal lattice passescompletely through the material. Multiple repetitions of this process along many planessimilar to A-A′ allow a metal to yield to an applied stress without fracturing. This ripplein the lattice structure is called a dislocation, and it is responsible for the ductile behaviorof metals.
Metals can be hardened and strengthened by a variety of treatments that make it moredifficult for dislocations to move through the metal lattice. Alloying, cold-working, andformation of second phases in a metal are all ways of impeding dislocation motion. Somecrystal structures of metals, such as intermetallic compounds, make it difficult fordislocations to move. The passage of a dislocation through the ordered structure of anintermetallic compound would result in an unfavorable atomic arrangement, sodislocations move only with difficulty.With metals, it is important to remember that their ability to yield without fracturing, aswell as all of the methods for making metals harder and stronger, is understandable inlight of the concept of dislocations in the metal structure.Other properties of metals, such as their electrical and thermal conductivity, can beunderstood as resulting from the metallic bond. In the metallic bond some of theelectrons are free to move rapidly through the lattice of metal ions. This unusual aspect ofthe metallic bond enables metals to conduct heat and electricity.The electronic structure of the metallic bond also accounts for the opacity of metals.Figure 1-8 illustrates the metallic bond with its lattice of positively charged metal ioncores and electrons that are free to move between the ion cores.Fig 1-8 Representation of the metallic bond showing the metal ion cores surrounded byfree electrons. (After Lewis and Secker, 1965.)
Dislocations in ceramic materials and in intermetallic compoundsWhy do ceramic materials not yield in the same manner as metals? The answer to thisquestion involves consideration of two types of ceramic materials:1. Amorphous materials (glasses)Glassy materials do not possess an orderedcrystalline structure as do metals. Therefore, dislocations of a crystalline lattice cannotexist in glassy materials. Thus, glasses have no mechanism for yielding without fracture.2. Crystalline ceramic materialsDislocations exist in crystalline ceramic materials, buttheir mobility is severely limited, because their movement would require that atoms oflike charge be brought adjacent to one another, as seen in Fig 1-9. The energy required todo this is so large that dislocations are essentially immobile in crystalline ceramicmaterials.Intermetallic compounds, unlike ordinary metal alloys, have a specific formula (eg,Ag3Sn, the main component of dental amalgam alloy powder) and an orderedarrangement of atoms. The movement of a dislocation through this ordered structurewould produce a disruption of the order similar to that shown in Fig 1-9 for crystallineceramic materials. Hence, dislocations move only with difficulty in intermetalliccompounds, and this property renders them more brittle than ordinary metal alloys.
Fig 1-9 The alternating charges of an ionic structure (crystalline ceramic) do not allowdislocations to move along plane A-A′. If a dislocation were to pass through such astructure, it would result in ions of like charge coming into direct contact, which wouldrequire too much energy.Clinical applications of metalsMetals are generally ductile and tough when compared to ceramics, although a few typesof metals, such as dental amalgams, are markedly more brittle than others. This ductilityallows the margins of castings to be burnished, orthodontic wires to be bent, and partialdenture clasps to be adjusted. Figure 1-10 shows how the ductility of metal allows thewire clasp for a partial denture framework to be bent permanently to provide the desiredretention. The ductile behavior of the partial denture alloy can be contrasted with thebrittle behavior of the intermetallic material, dental amalgam, as shown in Fig 1-11.
Fig 1-10 Ductility of metal as illustrated by the adaptation (bending) of a partial denturewrought wire clasp.Fig 1-11 Brittle fracture of an amalgam post and core that had supported a PFM crown.Set dental amalgam is a mixture of several intermetallic compounds. Intermetalliccompounds tend to be brittle rather than ductile. (Photo courtesy of R. P. OConnor,DMD.)
PolymersIntroductionThe behavior of polymers is fundamentally different from both ceramics and metals. Tounderstand this difference, it is useful to consider the modulus of elasticity and thestrength of polymers at a molecular level.Modulus of elasticityWhen chains of polyethylene are aligned parallel to one another and are subjected to atensile stress along their long axes (Fig 1-12(a)), the stress required to stretch the atoms inthe chains farther apart is surprisingly high. In fact, the modulus of elasticity ofpolyethylene when measured in this way is 30 million psi, about the same as steel!However, if the applied stress is perpendicular to the long axes of the chains (Fig 1-12(b)), the modulus of elasticity is only about 0.5 million psi. The high modulus ofelasticity (30 million psi) in the first case results from the strong bonds between the atomswithin polymer chains. The low elastic modulus (0.5 million psi) in the second caseresults from the weak bonds between atoms in adjacent chains.Bulk polymers have their polymer molecules in a more random, tangled arrangement, andhence there are somewhat fewer secondary bonds between chains than when the chainsare perfectly aligned. The tangling and coiling of the polymer molecules make polymerseven more flexible, because of the lower stress required to straighten out a coiledmolecule compared to the stress necessary to stretch the atoms in a molecule farther apart.
Fig 1-12 (a) Strong (primary) bonds between atoms within a polymer chain result in ahigh stiffness (modulus of elasticity) when aligned chains are stretched along theirlengths. (b) Weak (hydrogen) bonds between atoms in adjacent chains result in a lowmodulus of elasticity when aligned chains are stretched perpendicular to their lengths.StrengthThe low strength of polymers when compared to ceramics and metals can also beunderstood in terms of the strong bonds within polymer chains and the weak bondsbetween polymer chains. If the rule-of-thumb value for theoretical strength, 0.1E, isapplied to the oriented polyethylene fiber shown in Fig 1-12(a), a value of 3 million psi isobtained for the theoretical strength of polyethylene. Typical bulk polymers, however,seldom have tensile strengths of more than 10,000 psi. The weak secondary bondsbetween polymer chains allow these chains to slide past one another at much lowerstresses than those required to break the bonds within the chains.Thermal expansionThe increase of the temperature of a material as the result of increased atomic vibrationwithin it is a familiar concept. This atomic vibration is limited by the bonds betweenatoms in a material such that when strong bonds are present between atoms, the atoms
vibrate over a small amplitude, and when weak bonds are present, the atoms vibrate overa large amplitude. Ceramics and metals are characterized by strong bonds between atoms,and the secondary bonds play an insignificant role in their properties. As a result, mostceramics and metals expand relatively little when heatedthat is, their coefficients ofthermal expansion are relatively low. Polymers, however, are characterized by strongbonds within polymer chains and weak bonds between polymer chains. Thus, thevibration of carbon atoms within the polymer chain is restricted in the directions parallelto the long axis of the chain, but the atoms are free to vibrate in the two directionsperpendicular to the long axis of the polymer chain. As a result, when a polymer isheated, the chains must move farther apart to allow for the larger-amplitude vibration,which occurs perpendicular to the long axes of the polymer chains. This phenomenonaccounts for the large coefficient of thermal expansion exhibited by polymers. Figure 1-13 illustrates the different thermal expansion behaviors of a polymeric material and acrystalline material.Fig 1-13 The different thermal expansion behaviors of a polymeric material and acrystalline material.Water absorptionBecause of the weak secondary bonds in polymer materials, water molecules are able topenetrate between the polymer chains in a process called water absorption. Waterabsorption has both positive and negative aspects. On the positive side, it is the mainfactor in correcting the 0.5% processing shrinkage that occurs during the fabrication ofheat-cured denture bases. When the acrylic polymer absorbs water, the polymermolecules are forced apart slightly, causing the denture base to expand. This expansionduring water absorption compensates for the processing shrinkage.On the negative side, water is responsible for the hydrolytic degradation of polymers. Inaddition, the ions carried by the water may cause the polymer to break down morequickly or to become stained or malodorous.
Effect of cross-linkingBecause many of the undesirable properties of polymers are due to weak bonds betweenpolymer chains, it would seem that a way to improve them would be to link chainstogether with primary chemical bonds. In fact, this method, called cross-linking, iswidely used to improve strength, resistance to water absorption, abrasion resistance, andother properties of polymers. Because of the small number of primary bonds in a givenvolume of polymer material as compared to ceramics or metals, however, polymerproperties remain generally inferior even with cross-linking.The key to understanding polymers is that the low strengths and elastic moduli ofpolymers, as well as many other distinctive properties, can be seen in light of the conceptof strong bonds within polymer chains and weak bonds between polymer chains.Clinical applications of polymersPolymers have had limited use as restorative materials by themselves because of their lowstrength and high thermal expansion. Some of the unfavorable properties of polymershave been mitigated by the incorporation of inorganic fillers to form composite materials.Modification of the polymer resins themselves to make them hydrophobic has improvedtheir resistance to water absorption. The properties of polymers may be further improvedby increasing their crystallinity, but the bonds between chains in crystalline polymers arestill only secondary bonds. The intrinsic weaknesses of polymers will probably continueto limit their use as restorative materials. The incisal fracture of a Class 4 microfilledcomposite restoration is shown in Fig 1-14. Microfilled resin composites tend to haveconsiderably lower levels of the stronger inorganic filler, and so the stresses are bornemore heavily by the weaker resin matrix. In Class 4 restorations, microfills generally haveinsufficient strength to withstand the stresses that may be encountered.Fig 1-14 Fracture of a Class 4 microfilled composite restoration. The low filler content ofmost microfills leaves the polymer matrix bearing the majority of the stress. Polymers aregenerally too weak for bearing large stresses. (Photo courtesy of C. D. Smith, DDS.)Glossaryalloy A material that exhibits metallic properties and is composed of one or moreelementsat least one of which is a metal. For example, steel is an alloy of iron and
carbon, brass is an alloy of copper and zinc, and bronze is an alloy of copper and tin.amorphous Literally, "without form." Atoms in crystalline solids exhibit an orderedarrangement, whereas atoms in amorphous solids lack this long-range periodicity.ceramic In the broadest sense, a compound of metallic and nonmetallic elements. By thisdefinition, materials ranging from aluminum oxide (Al 2O3) to table salt (NaCl) areclassified as ceramics. In dentistry, gypsum (CaSO 4 ⋅ 2H2O), many dental cements (eg,zinc phosphate), and porcelains are examples of ceramic materials.cross-linking A method for making a polymer stronger and more rigid by creatingchemical bonds between the molecular chains in the polymer.crystalline Having atoms or molecules arranged in a regular, repeating three-dimensionalpattern. Metals are nearly always crystalline; ceramics and polymers can be crystalline ornoncrystalline (amorphous).dislocation A defect in a crystal that is caused by an extra plane of atoms in the structure(see Fig 1-7). The movement of dislocations is responsible for the ability of metals tobend without breaking.intermetallic compound A chemical compound whose components are metals. Thegamma phase of amalgam, Ag3Sn, is an example of an intermetallic compound.metal A crystalline material that consists of positively charged ions in an ordered, closelypacked arrangement and bonded with a cloud of free electrons. This type of bond, called ametallic bond, is responsible for many of the properties of metalselectrical and thermalconductivity, metallic luster, and (usually) high strength.metallic bond One of the three types of primary (strong) chemical bond. (Ionic andcovalent are the other two.) Metallic bonds involve the sharing of valence electronsamong all atoms in the metal. Metallic bonds are responsible for many of the distinctiveproperties of metals, including electrical conductivity.modulus of elasticity A measure of the stiffness or flexibility of a material. A stiffmaterial has a high modulus of elasticity, and a flexible material has a low modulus ofelasticity. Also called Youngs modulus. (See chapter 2 for more detail.)polymer A material that is made up of repeating units, or mers. Most polymers are basedon a carbon (-C-C-C-C-) backbone in the polymer chain, although a silicone (-O-Si-O-Si-O-) backbone is important in many polymers.stress raiser An irregularity on the surface or in the interior of an object that causesapplied stress to concentrate in a localized area of the object. Other things being equal,the sharper the stress raiser, the greater the localized stress around it.water absorption The penetration of water into the structure of a material. Waterabsorption by polymers can help offset the effects of processing or polymerizationshrinkage (as in heat-processed denture bases), but it can also have detrimental effects,such as discoloration and leaching of unreacted components. For water to be absorbedinto the structure of a material, it must first be adsorbed onto the surface. Because bothphenomena occur when water is absorbed, the process is often referred to simply as
Chapter 2. Physical Properties and BiocompatibilityIntroductionPhysical properties determine how materials respond to changes in their environments,and biocompatibility relates to the effect a material has on the tissue it contacts. Therelationships among the various properties are classified according to the scheme in Fig2-1.Fig 2-1 A tree diagram classifying physical properties.Mechanical PropertiesIntroductionThe concepts of stress, strain, modulus of elasticity, plastic deformation, and otherproperties were introduced in chapter 1. Because of the unfamiliarity and abstruse nature
of many of these concepts, they will be discussed here in somewhat greater depth, andsome additional concepts will be introduced as necessary to understand the physicalbehavior of materials.StressConsider again the block of material described in the previous chapter that was 1/2 in ×1/2 in (1.27 cm × 1.27 cm) in cross section and was subjected to a 3,000-lb (about 13 kN)load. As was pointed out in that example, the stress experienced by thatblockdetermined by dividing the force by the cross-sectional area of the blockis12,000 psi, or 83 MPa. Stress (σ) is the force (F) divided by the cross-sectional area (A):Now consider a similar block, but with smaller dimensions1/4 in × 1/4 in (about 0.6 cm× 0.6 cm) in cross section (area of 1/16 in 2, or about 0.4 cm2). If this new block issubjected to the same 3,000-lb (13-kN) tensile load, the stress in this case is 3,000 lb (13kN) divided by 1/16 in2 (about 0.4 cm2) = 48,000 psi (about 330 MPa).Thus, the usefulness of the concept of stress is apparent. It is not sufficient merely to statethe load or force that is being applied to a dental material, because the stress that isproduced in the material depends just as much on the cross-sectional area on which theload is acting as it does on the load itself. For instance, if the block that measured 1/4 in ×1/4 in in cross section is subjected to a load of 12,000 lb (about 53 kN) instead of 3,000 lb(about 13 kN), the stress is 48,000 psi (about 330 MPa). If the cross-sectional area ismade 4 times smaller (1/4 as large), or if the load is made 4 times larger, the stress isincreased by a factor of 4. Thus, the stress is said to be inversely proportional to the cross-sectional area and directly proportional to the load.The basic types of stresses produced in dental structures under a force are tensile,compressive, and shear. All three are present in a beam loaded in the center. If the valueof these stresses exceeds the strength of the material, the structure will fail. It is thereforeimportant to know the strength values of materials. It is rare that an object will be subjectto the pure tensile, compressive, or shear stresses experienced by test specimens in amaterials testing laboratory. As shown in Fig 2-2, however, wherever bending forces arepresent, tensile stresses are present in critical areas, which could result in failure.
Fig 2-2 (a) Tensile stress (ST) at the isthmus of a two-surface amalgam restoration. (b)Tensile stress at the occlusal surface of a beveled amalgam restoration. (c) Tensile stressat the junctions of a partial denture clasp. (d) Tensile and compressive stresses (S C) in asoldering bridge. F = force; A = area. (From Mahler and Terkla, 1958. Reprinted withpermission.)StrainWhen a block of material is subjected to a tensile stress as described in the precedingsection, it temporarily becomes longer by a certain amount. This temporary increase inlength is called strain. A few examples will illustrate how strain is described. Considerthe block with the cross section of 1/4 in × 1/4 in = 1/16 in2 (0.6 cm × 0.6 cm = 0.4 cm2)and assume it has a length of 10 in (25.40 cm) when no load is applied. If the length ismeasured while the 3,000-lb (13-kN) load is being applied and the new length is 10.016in (25.441 cm), the strain is computed by dividing the increase in length (0.016 in, 0.041cm) by the original length (10.000 in, 25.40 cm) to obtain 0.0016. Strain is adimensionless quantity because we are dividing unit length by unit length, but sometimesit is written as "in/in" or "cm/cm." Strain can also be expressed in a percentage, in whichcase the dimensionless value is multiplied by 100%. In the given example, the strainwould be 0.16%.If a piece of the same material with the same cross section but 11 in (27.940 cm) longwere subjected to the same load (3,000 lb, about 13 kN), and the length of the block of
material were measured while the load was being applied, it would be 11.0176 in(27.9847 cm). To compute the strain produced, the change in length (0.0176 in, 0.0447cm) is divided by the original length (11.0000 in, 27.9400 cm); the strain is determined tobe 0.0016 (or 0.16%), the same value obtained above for the block of material measuring10 in (25.4 cm). Thus, it can be seen that strain is independent of the length of thespecimen.Now consider a bar of high-strength steel, 1/4 in × 1/4 in = 1/16 in2 (0.6 cm × 0.6 cm =0.4 cm2) in cross section and 10 in (25.4 cm) long, that is capable of supporting a tensileload of 6,000 lb (about 27 kN). If the length of this bar were measured while under this6,000-lb (27-kN) load, it would be 10.032 in (25.4813 cm). If the strain is computed asbefore, the change in length (0.032 in, 0.0813 cm) divided by the original length (10.000in, 25.4 cm) is found to be 0.0032 or 0.32%. Hence, it can be seen that if the cross-sectional area of the block of material is kept the same and the applied load is doubled,the strain experienced by the material is doubled.ElasticityThe preceding examples showed that both stress and strain are directly proportional to theload applied when the cross-sectional area is kept the same. Hence, if the load is doubled,both the stress and the strain likewise will be doubled. It can be seen that the ratiobetween stress (σ) and strain (ε) is the same, thus:The property of having a constant ratio of stress to strain is called elasticity, and theconstant that is the ratio of stress to strain is called the modulus of elasticity. To gain aclearer understanding of the concept of elasticity and to see what it means for twomaterials to have different moduli of elasticity, it is helpful to consider the analogy of twosprings of different stiffnesses, as shown in Fig 2-3. Spring 2 is stiffer than spring 1;therefore, when they support equal weights, the stiffer spring is extended a smalleramount. Increasing the load from 1 lb (4.4 N) to 2 lb (8.9 N) causes each spring to extendtwice as much as it did under the 1-lb (4.4-N) load. Subjecting both springs to a 3-lb (13-N) load causes each one to extend 3 times as much as it did under a 1-lb (4.4-N) load, andso on. It can be seen that, irrespective of the load applied for either spring 1 or spring 2,the ratio of the extension to the load is a constant for that spring. However, the constantsfor the two springs are different. In this analogy, the extension of the spring correspondsto strain, the load or weight on the spring corresponds to stress, and the spring constantcorresponds to the modulus of elasticity.It is obvious that more weight cannot be added to a spring indefinitely and still have theextension increase proportionately. At some point the spring will become "stretched out"and will not return to its original size when the weight is removed. In the same way, whena material is stressed above a certain point, stress is no longer proportional to strain. Thehighest stress at which stress is proportional to strain is called the elastic limit, or theproportional limit. Because this stress is difficult to determine precisely, as it wouldentail looking for an infinitely small deviation from proportionality, it is customary todesignate a certain permanent deformation or offset (usually 0.002, or 0.2%) and to reportthe yield strength of the material at this strain. Thus the terms "elastic limit" and"proportional limit" are synonymous, whereas "yield strength" has a slightly differentmeaning. The yield strength of a material is always slightly higher than the elastic limit.
If a material continues to have more and more weight applied to it, it will of courseeventually break. If the material is being stretched (tensile loading), the stress at breakageis called the ultimate tensile strength (UTS). When many metals are stressed above theirproportional limits, they undergo a process called work hardening, and actually becomestronger and harder. But with the increased strength provided by work hardening comesincreased brittleness. It is thus very important to avoid overdoing it when bending a wireor a partial denture clasptoo much bending of the metal back and forth will make itharder and more brittle.The modulus of elasticity is an inherent property of the material and cannot be alteredappreciably by heat treatment, work hardening, or any other kind of conditioning. Thisproperty is called structure insensitivity, because it is not sensitive to any alteration to thestructure (meaning the microstructure) of the material. The modulus of elasticity is one ofthe few properties that is not sensitive to any alteration of the structure of the material.The yield strength of a material, for example, is sensitive to work hardening and willincrease with increasing amounts of work hardening.Fig 2-3 The concept of modulus of elasticity using the analogy of springs. Spring 1 is aflexible spring, representing a material with a low modulus of elasticity. Spring 2 is a stiffspring, representing a material with a high modulus of elasticity. When the same load is
applied to both springs, they stretch different amounts. The weight applied to the spring isanalogous to the stress (σ), the amount the spring stretches is analogous to the strain (ε),and the stiffness of the spring is analogous to the modulus of elasticity (E).PlasticityWhen the elastic or proportional limit is exceeded in a material, it is said to exhibit plasticbehavior. (The term "plastic" means "moldable," but the term has come to be associatedwith polymers.) Materials that experience a large amount of plastic behavior orpermanent deformation are said to be ductile. Materials that undergo little or no plasticbehavior are said to be brittle. If stress is plotted against strain, with stress as the ordinate(y axis) and strain as the abscissa (x axis), a diagram such as the one in Fig 2-4 is theresult. It can be seen that stress is proportional to strength up to the elastic (orproportional) limit. Above this stress, stress and strain are no longer proportional. If amaterial is stressed into the plastic region or region of permanent deformation and thenthe stress is removed, the material will have a permanent set, or deformation. If stress iscontinuously increased, the material will undergo more and more plastic deformation andwill ultimately fracture. The highest stress achieved during this process is called theultimate tensile strength of the material, as mentioned previously. The total strain atfracture (elastic strain + plastic strain) is called the elongation. Elongation of metals isimportant in several situations in dentistry. When one is burnishing the margin of acrown, the property that most comes into play is the elongation, although the yieldstrength is also important. For example, gold alloys are generally easy to burnish becausethey have a lower yield strength. Nickel-chromium and cobalt-chromium alloys may haveadequate elongation for burnishing, but their yield strengths are so high that they makeburnishing difficult. Another example of the importance of elongation is the bending of apartial denture clasp to adjust the retention.The entire area under the stress-strain curve is a measure of the energy required tofracture the material, or its toughness. The area under only the elastic region of the stress-strain curve is a measure of the ability of the material to store elastic energy (the way acompressed spring does). This is called the resilience of the material.Tabulated data for (Youngs) modulus of elasticity, yield strength, ultimate tensilestrength, percent elongation, and other mechanical properties are listed in Appendix A.
Fig 2-4 Measurement of stress and strain on an object being stretched. In the regionlabeled "elastic deformation," stress is proportional to strain, whereas in the regionlabeled "plastic deformation," stress and strain are no longer proportional (strain increasesfaster than stress does). The highest stress at which stress and strain are still proportionalis called the proportional limit, and the maximum stress just before the object breaks iscalled the ultimate tensile strength. The total amount that the object stretches (ie, the totalstrain), which is the sum of the elastic deformation and the plastic deformation, is calledthe percent elongation.FatigueWhen materials are subjected to cycles of loading and unloading, as during mastication,they may fail due to fatigue at stresses below the ultimate tensile strength. Usually, smallcracks at the surface or within the material gradually grow larger upon cycling, andeventually the material fails. Fatigue curves, such as the one shown in Fig 2-5, show theexperimentally determined number of cycles to failure at different stress levels. Thehigher the stress placed on and off the material, the fewer the number of cycles untilfailure.
Fig 2-5 Fatigue curves for glass-filled resin composite restorative material. (Courtesy ofR. A. Draughn, PhD.)Viscous flowMany dental materials are in a fluid state when they are formed, and viscous flowphenomena are important considerations. Our understanding of the behavior ofimpression materials and amalgam involve viscoelastic phenomena. When shear stress-strain rate (flow rate) plots are obtained, they enable viscous materials to be classified inseveral ways. A newtonian fluid shows a constant viscosity, η, which is independent ofstrain rate:where η is the viscosity in poise, σ is the shear stress acting on the fluid, and ε is thestrain, or flow rate.Actual fluids differ from these in their flow responses to the level of stress applied. Plasticfluids (eg, putty) dont flow at all until a minimum stress is applied. Pseudoplastic fluids(eg, fluoride gels) show an instantaneous decrease in apparent viscosity or consistency(become more free-flowing) with increasing shear rate. Dilatant fluids (eg, fluid denturebase resins) show an increase in rigidity as more pressure is applied. Thixotropic fluids(eg, fluoride gels, house paints) flow more freely when vibrated, shaken, or stirred than ifallowed to sit undisturbed. Formulation of the various suspensions and gels used indentistry to impart one or more of these properties can make them easier to handle. Forexample, impression materials that do not run off impression trays but are less viscousunder pressure in a syringe have a definite advantage.Viscoelastic behaviorMany materials, including elastic impression materials, waxes, and even hardenedamalgam, show a combination of elasticity and viscous flow. Figure 2-6 is a model ofhow a viscoelastic material acts under stress, the so-called spring-and-dashpot (or Voigt)
model. (A dashpot is an oil-filled cylinder with a loosely fitted pistonmost automobileshock absorbers are of a dashpot design.) As the model is stretched, the spring componenton the left stretches and the piston of the dashpot also moves through the viscous liquid.The strain under stress and after release of the stress is time-dependent. The straingradually builds up until the release of stress, and then it gradually goes back to zero asthe spring element returns to its original length but is dampened by the dashpot element.Elastic impression materials are viscoelastic; initially they are strained upon removalfrom the mouth and require a short period of time to recover before models or dies arepoured.Fig 2-6 (a) Voight model for viscoelastic behavior. (b) Response of (a) to stress. Strainincreases with time and decreases after force (F) is released at t 1, but is slow due to thedamping effect of the dashpot or the elastic action of the spring element. (From OBrienand Ryge, 1978. Reprinted with permission.)HardnessThe resistance of a material to indentation or penetration is called hardness. Thetechnical definition of hardness varies little, if at all, from the familiar definition, with thepossible exception that the technical definition carries with it the connotation of a methodof measurement. Most of the methods for measuring hardness consist of making a dent inthe surface of a material with a specified force in a controlled and reproducible mannerand measuring the size of the dent. For the measurement methods discussed in thissection, as the hardness increases, the respective hardness number increases also. Forexample, Fig 2-7 indicates the relative positions of a variety of dental and other materialson a Knoop hardness scale ranging from soft on the left to hard on the right. The positionsof the different materials on the line indicate their relative hardnesses.Brinell hardness number (BHN)The indenter for the Brinell hardness test is a small, hardened steel ball, which is forced
into the surface of a material under a specified load. This indentation process leaves around dent in the material, and hardness is determined by measuring the diameter of thedent. Brinell hardness values for selected metals are listed in Appendix A.Vickers hardness number (VHN) or diamond pyramid hardness (DPH)The Vickers hardness indenter is a square, pyramid-shaped diamond, which leaves asquare, diamond-shaped indentation in the surface of the material being tested. Hardnessis determined by measuring the diagonals of the square and taking the average of the twodimensions. The Vickers hardness test is also called the diamond pyramid hardness test.The Brinell and Vickers hardness tests are both used to measure the hardness of dentalalloys, and hardness values on alloy packages are expressed in either Vickers or Brinellhardness numbers. To compare Vickers and Brinell numbers, use the followingrelationship:For example, if a package of casting alloy lists a Vickers hardness of 242 and you want tocompare it with a different brand that lists the Brinell hardness, you would divide theVHN by 1.05 to obtain a BHN of 230. Diamond pyramid (Vickers) hardness values forseveral types of materials are listed in Appendix A.Knoop hardness (KHN)The indenter for the Knoop hardness test is also made of a diamond, but its outline issomewhat different from the Vickers indenter; although it is diamond shaped, onediagonal is much longer than the other. Only the long diagonal is measured to determinethe Knoop hardness number. Knoop hardness numbers for a variety of materials are listedin Appendix A.Rockwell hardness (RA, RB, . . . RG)The Rockwell hardness test is used primarily for determining the hardnesses of steels andis the most widely used hardness test in the United States. The Vickers, Brinell, andKnoop hardness tests are more commonly used for dental materials, however. Rockwelluses different hardened steel balls or diamond cones and different loads. Eachcombination forms a specific Rockwell scale (A, B, and C scales are the most common).The different scales are used for materials of different hardness ranges.Shore A durometerThe Shore A hardness test is used to measure the hardness of rubbers and soft plastics.The Shore A scale is between 0 and 100 units, with complete penetration of the materialby the indenter yielding a value of 0, and no penetration yielding a value of 100. Shore Ahardness values for several polymeric materials are listed in Appendix A.
Fig 2-7 Relative hardnesses of a variety of dental materials and tooth substances.Thermal PropertiesHeat flow through a materialMetals tend to be good conductors of heat, and this property must be taken intoconsideration when placing metallic restorations. Dentin is a thermal insulator (poorconductor of heat); thus, when a sufficient thickness of dentin is present, the patient feelsno sensitivity to heat and cold through a metallic restoration. However, when only a thinlayer of dentin remains, some thermal protection must be provided for the pulp. A goodrule of thumb in determining the thickness of cement base necessary in a given situationis to visualize how much dentin would have to be present in the excavation site so no basewould be necessary and then to apply base up to this level. The rate at which heat flowsthrough a material is expressed as thermal conductivity or thermal diffusivity. Thedifference between these two terms is described in the following subsections.Thermal conductivityThermal conductivity (k) is a measure of the speed at which heat travels (in calories persecond) through a given thickness of material (1 cm), when one side of the material ismaintained at a constant temperature that is 1°C higher than the other side. Thermalconductivity is expressed in units of cal/cm ⋅ sec ⋅ °C. Thermal conductivity values for avariety of materials are listed in Appendix A.Thermal diffusivityWhereas thermal conductivity gives an idea of the relative rates at which heat flowsthrough various materials, it fails to take into account the fact that various materialsrequire different amounts of heat (calories) to raise their temperatures an equal amount.For example, 1 gram of water requires 1.000 calorie to raise its temperature 1°C, whereas1 gram of dentin requires only 0.28 calorie, and 1 gram of gold requires only 0.031calorie to produce a 1°C temperature increase. Thus, thermal conductivity alone will nottell us, for instance, how rapidly the interior surface under a crown will heat up when theexterior surface is heated. To know how quickly the interior of the crown will approach
the temperature of the exterior, we need to know the thermal diffusivity of the alloy. Thethermal diffusivity (h) of a material (expressed in units of mm 2/sec) is dependent on itsthermal conductivity, heat capacity (C p), and density (ρ):The relative thermal diffusivities of several dental materials are shown in Fig 2-8, andtabular data on a variety of materials are included in Appendix A.Fig 2-8 Thermal diffusivities of restorative materials.Thermal expansionThere are several situations in dentistry in which the thermal expansion of materials isimportant. Some restorative materials have coefficients of thermal expansion that aremarkedly different from tooth structure. In such cases, temperature fluctuations that occurin the mouth can cause percolation at the tooth-restoration interface as the restorationcontracts and expands. The porcelain and metal in a porcelain-fused-to-metal (PFM)restoration must contract at the same rate upon cooling from the porcelain firingtemperature if the buildup of large residual stresses is to be avoided. The cooling of adenture base from the processing temperature to room temperature is primarilyresponsible for the processing shrinkage that occurs. The thermal expansion behavior ofdental wax, gold alloy, investment, and so on are all important in producing properlyfitting castings. Figure 2-9 illustrates the relative values of linear coefficient of thermalexpansion for tooth, amalgam, composite, and acrylic resin. The diagram is onlyschematicthe expansion has been magnified to make it visible; the actual thermalexpansion would be too small to see. The thermal expansion coefficients, or the fractionalchanges in length per degree celsius, are given in parentheses. Tabular thermal expansiondata on a variety of materials are included in Appendix A.
Fig 2-9 Relative thermal expansions of several restorative materials and tooth structure.The relative amounts the materials expand when heated the same amount are representedby the dashed lines. The amount of expansion is magnified to make it visible forcomparison of the materials.Electrical and Electrochemical PropertiesElectrode potentialsAn electrochemical series is a listing of elements according to their tendency to gain orlose electrons in solution. The series is referenced versus the potential of a standardhydrogen electrode, which is arbitrarily assigned a value of 0.000 volts. If the elementsare listed according to the tendency of their atoms to lose electrons, the potentials aretermed oxidation potentials. If they are listed according to the tendency of their ions togain electrons, the potentials are termed reduction potentials. Reduction potentials at25°C and 1 atmosphere of pressure are termed standard electrode potentials (Table 2-1). Table 2-1 Standard electrode potentialsHalf-reaction E0 (volts)Li+ + e = Li -3.04K+ + e = K -2.93 2+Ca + 2e = Ca -2.87 +Na + e = Na -2.71Mg2+ + 2e = Mg -2.37 3+Al + 3e = Al -1.662 2+Zn + 2e = Zn -0.762 3+Cr + 3e = Cr -0.744Fe2+ + 2e = Fe -0.447 2+Ni + 2e = Ni -0.257 2+Sn + 2e = Sn -0.1375Pb2+ + 2e = Pb -0.1262 3+Fe + 3e = Fe -0.037 +H +e=H 0.000 (reference)Cu2+ + 2e = Cu +0.342
Cu+ + e = Cu +0.521Ag+ + e = Ag +0.800Hg2+ + 2e = Hg +0.851Pt2+ + 2e = Pt +1.118Au+ + e = Au +1.692Metals with a large positive electrode potential, such as platinum and gold, are moreresistant to oxidation and corrosion in the oral cavity. If there is a large differencebetween the electrode potentials of two metals in contact with the same solution, such asbetween gold and aluminum, an electrolytic cell may develop. If this occurs in the mouth,the patient may experience discomfort.The exact nature of tarnish and corrosion of restorative materials in vivo is extremelycomplex and involves much more than electrode potentials of materials. A possiblesource of the corrosion of gold alloys is accidental contamination of the surface withcopper during pickling, and subsequent tarnishing in saliva (Fig 2-10).Fig 2-10 Accidental plating of copper during pickling of gold casting. The model of thecell is formed by iron tongs and gold alloy (right). (From OBrien, 1962. Reprinted withpermission.)Electrical resistivityElectrical resistivity measures the resistance of a material to the flow of an electricalcurrent. The relationship between the resistance (R) in ohms, the resistivity (ρ), the length(l), and the cross-sectional area (A) is as follows:Electrical resistivity values for several materials are given in Table 2-2.
Table 2-2 Electrical resistivity of several materialsMaterial Resistivity (ohm-cm)Copper 1.7 × 10-6SiO2 (glass) > 1014Human enamel ~4 × 106Human dentin ~3 × 104Zinc phosphate cement 2 × 105Zinc oxide-eugenol 5 × 109 The low resistivity of metallic restorative materials is responsible for discomfort to thepulp if dissimilar metals generate a voltage. The insulating properties of cements help toreduce this problem.BiocompatibilityA material that is designed to be implanted in the body for the repair or replacement of adiseased or damaged tissue is called a biomaterial. Biomaterials must be biocompatible.All materials used in medicine and dentistry interact with tissues, producing changes inboth the materials and the surrounding tissues; there is no such thing as an "inert"material.Several factors affect the biocompatibility of a material. The chemical composition andstructure of the material affect the type and quantities of chemical species released. Therelative abundance of chemical species in a material will not reliably predict the amountsor even the proportions of the chemical species released. For this reason, thebiocompatibility of a material is usually determined empirically. The characteristics of thesite of use also affect a materials biocompatibility. For example, the presence of manyfactors in the oral environment affect the release of components from dental materials.Chemical factors, such as bacterial metabolic products, water, enzymes, and polar andnonpolar solvents, can accelerate the release of components. Mechanical factors in thesite of use can also affect the biocompatibility of a material. For example, under mostconditions, high-molecular-weight polyethylene elicits little if any tissue reaction whenimplanted. When it is used for the acetabular (socket) side of a total hip replacement,however, it can generate wear debris over time that produces an inflammatory responsethat eventually causes loosening of the prosthesis and failure of the implant.Evidence on a new product for use in the body must first be presented to governmentagencies that document possible adverse reactions the material might cause. Thisinformation includes the history of the material, its chemical composition, and resultsfrom a series of biocompatibility tests. A product that is a new version of an oldcomposition used successfully in similar applications may be classified under the FederalDrug Administration (FDA) classification of 510(k), which requires less extensive testingfor premarket approval. Another strategic qualification is whether the new product hastemporary or long-term contact with the body. The FDA has different categories formaterials with short-term contact, such as an impression material, than for materials usedfor long-term service, such as a cemented crown or an implant. The more potential forharm, the greater the burden of testing required. The testing required depends on manyfactors, including the results of initial minimal screening tests. A brief description ofthese tests is provided in Appendix B.
Glossarybiocompatible A material is considered biocompatible if it does not produce harmful ortoxic reactions in the tissues it contacts or adverse systemic reactions as a result ofelements, ions, and/or compounds it releases.biomaterial A material that is designed to be implanted in the body for the repair orreplacement of a diseased or damaged tissue.brittle A material that tends to fracture without appreciable plastic deformation is said tobe brittle.compressive stress Two forces applied toward one another in the same straight line.ductility Ability of a material to be plastically strained in tension.elasticity Ability to sustain deformation without permanent change in size or shape.electrical resistivity Ability of a material to resist conduction of an electric current.elongation Overall deformation (elastic + plastic) as a result of tensile force application.fatigue Tendency to fracture under cyclic stresses.hardness Resistance to permanent indentation on the surface.linear coefficient of thermal expansion Change in length per unit original length for a1°C temperature change.modulus of elasticity Stiffness of a material within the elastic range. Numerically, it isthe ratio of stress and strain.percolation The pumping of oral fluids in and out at the tooth-restoration interface as therestoration contracts and expands with temperature changes. Percolation occurs when thethermal expansion coefficient of the restoration is markedly different from that of toothstructure.proportional limit (elastic limit) The maximum stress at which the straight-linerelationship between stress and strain is valid.resilience Energy needed to deform a material to the proportional limit.shear stress Two forces applied toward one another but not in the same straight line.strain (nominal) Change in length per unit original length.stress (nominal) Force per unit area.tensile stress Two forces applied away from one another in the same straight line.thermal conductivity The quantity of heat passing through a material 1 cm thick with a
cross section of 1 cm2, having a temperature difference of 1°C.thermal diffusivity Measure of the heat transfer of a material in the time-dependent state.toughness Amount of energy needed for fracture.ultimate tensile strength The maximum strength obtained based on the originaldimensions of the sample.viscoelastic Having both elastic and viscous properties.viscous Resistant to flow (referring to a fluid).work hardening The increase in strength and hardness, with accompanying decrease inductility, that occurs in a ductile metal as it is plastically deformed. Also called strainhardening.yield strength Strength measured at the stress at which a small amount of plastic strainoccurs. Also called yield point.Discussion Questions1. What is galvanic action in the mouth and how can it be minimized?2. Why is thermal diffusivity more relevant to insulation of the pulp than thermalconductivity?3. Explain why fixed partial dentures may fail under tensile stresses when under bitingforces that appear to be compressive?4. How is the leakage of oral fluids around a composite restoration related to thecoefficient of thermal expansion and temperature changes in the mouth?5. Why is time so important in the behavior of viscoelastic materials such as impressionmaterials and waxes?6. Why is there a hierarchy of biocompatibility tests?7. Why can biocompatibility tests be difficult to interpret?Study Questions(See Appendix E for answers.)1. Discuss why a knowledge and understanding of the physical and mechanical propertiesof biomaterials is important in dentistry.2. Explain why the thermal diffusivity of a material is more applicable to behavior in vivothan is its thermal conductivity.3. Draw and label a stress-strain diagram including the proportional limit, yield point, andultimate tensile strength.
4. Define hardness and its relation to other mechanical properties.5. Compare materials a and b on the basis of the two stress-strain curves below, obtainedby pulling the materials in tension.6. Why are laboratory biocompatibility tests run prior to clinical trials?Recommended ReadingASTM (1995). Practice for direct contact cell culture evaluation of materials for medicaldevices. Annual Book of ASTM Standards, 13.01, F813, 233-236.ASTM (1995). Standard test method for agar diffusion cell culture screening forcytotoxicity. Annual Book of ASTM Standards 13.01, F895, 247-250.Babich H, Borenfreund E (1987). Structure-activity relationship (SAR) modelsestablished in vitro with the neutral red cytotoxicity assay. Toxicol In Vitro 1:3-9.Billmeyer FW Jr (1984). Textbook of Polymer Science, ed 3. New York: John Wiley &Sons.Borenfreund E, Puerner JA (1987). Short-term quantitative in vitro cytotoxicity assayinvolving an S-9 activating system. Cancer Lett 34:243-248.Callister WD Jr (1999). Materials Science and Engineering: an introduction, ed 5. NewYork: John Wiley & Sons.Chappell RP, Spencer P, Eick JD (1994). The effects of current dentinal adhesives on thedentinal surface. Quintessence Int 25:851-859.Chiang Y-M, Birnie D III, Kingery WD (1997). Physical Ceramics. New York: JohnWiley & Sons.Dieter GE (1986). Mechanical Metallurgy, ed 3. New York: McGraw-Hill.
Doremus RH (1994). Glass Science, ed 2. New York: John Wiley & Sons.Ferracane JL, Condon JR (1990). Rate of elution of leachable components fromcomposites. Dent Mat 6:282-287.Hanks CT, Wataha JC, Sun Z (1996). In vitro models of biocompatibility: a review. DentMater 12:186-193.ISO (1992). "In vitro" method of test for cytotoxicity of medical and dental materials anddevices. Pforzheim, Germany: International Standards Organization, ISO/10993-5.Mahler DB, Terkla LG (1958). Analysis of stress in dental structures. Dent Clin NorthAm (Nov).OBrien WJ (1962). Electrochemical corrosion of gold alloys. Dent Abstracts 7:46.OBrien WJ, Ryge G (1978). Outline of Dental Materials. Philadelphia: WB Saunders.Rathbun MA, Craig RG, Hanks CT, Filisko FE (1991). Cytotoxicity of a bis-GMA dentalcomposite before and after leaching in organic solvents. J Biomed Mater Res 25:443-457.Ratner BD, et al (eds) (1996). Biomaterials Science: An Introduction to Materials inMedicine. San Diego: Academic Press.Reed-Hill RE, Abbaschian R (1991). Physical Metallurgy Principles. Boston: PWS-Kent.Tyas MJ (1977). A method for the in vitro toxicity testing of dental restorative materials.J Dent Res 56:1285-1290.Williams D (ed) (1990). Concise Encyclopedia of Medical and Dental Materials. Oxford:Pergamon Press.Chapter 3. Color and AppearanceIntroductionAmong the important factors that influence esthetic appearances of restorations are color,translucency, gloss, and fluorescence. Each of these factors, as perceived by an observersuch as a dentist, technician, or patient, is influenced by (1) the illuminant (light source),(2) the inherent optical parameters of the restorative materials that dictate the interactionof the light from the illuminant with the material, and (3) the interpretation of theobserver (Fig 3-1). An understanding of these factors in restorative materials, and properconsideration and communication of this information, will greatly assist the choice andfabrication of esthetic restorations.
Fig 3-1 Illuminant, object, and observer interaction.IlluminantIntroductionLight waves emitted from the illuminant interact with the object and are perceived by theobserver. The color content of the illuminant interacts with the object being perceived.The color content of the illuminant is the intensity of light emitted at each wavelength(spectral distribution). This is dependent on the type of illuminant. The wavelengths oflight are associated with hues, commonly referred to as color (Fig 3-2).Fig 3-2 Wavelength and hue. (Adapted from Billmeyer and Saltzman, 1960.)White light contains a mixture of wavelengths (colors). It is dispersed into componentswhen it passes through a prism, as shown in Fig 3-3.
Fig 3-3 Dispersion of white light by a prism.Different illuminants have different intensity distributions, or spectra, with respect towavelength, as illustrated in Figs 3-4a and 3-4b.Fig 3-4a Intensity distributions of illuminant A.
Fig 3-4b Intensity distributions of fluorescent light.Illuminants are sometimes described by their color temperature (in degrees Kelvin). Thisis based on the equivalence of the illuminant as compared to a radiating body with atemperature equal to the color temperature.The characteristics of an illuminant are important in color evaluation because the intensitydistribution, with respect to wavelength, identifies the light spectrum available to interactwith the object and then be perceived by the observer. In any color description the type ofilluminant used needs to be defined. Furthermore, the appropriate illuminant needs to beused in shade selection and shade matching. Illuminants that closely approximate daylightare preferred because color considerations for restorations, when seen under theseilluminants, are close to those seen under natural light. Several "daylight" sourcesintended for use in dental operatories are available. Representative spectral distributionsof some of these illuminants are shown in Figs 3-5a and 3-5b.